General

Property | Value | Condition | Related Standards |
---|---|---|---|

Density | 2.84 g/cm³ Show Material materials with Density of 2.84 g/cm³ | T851 | AA Standards, ASTM B209, ASTM B211 |

2.84 g/cm³ Show Material materials with Density of 2.84 g/cm³ | T851 | ||

3.1 g/cm³ Show Material materials with Density of 3.1 g/cm³ | T851 |

Mechanical

Property | Temperature | Value | Condition | Related Standards | Comment |
---|---|---|---|---|---|

Bending Fatigue Strength | 105.0 MPa Show Material materials with Bending Fatigue Strength of 105.0 MPa | T851 | AA Standards | ||

Creep strength | 24 °C | 420 MPa Show Material materials with Creep strength of 420 MPa | T851 | up to 1000 hours | |

100 °C | 315 MPa Show Material materials with Creep strength of 315 MPa | T851 | up to 1000 hours | ||

150 °C | 235 MPa Show Material materials with Creep strength of 235 MPa | T851 | up to 1000 hours | ||

175 °C | 185 MPa Show Material materials with Creep strength of 185 MPa | T851 | up to 1000 hours | ||

205 °C | 150 MPa Show Material materials with Creep strength of 150 MPa | T851 | up to 1000 hours | ||

230 °C | 125 MPa Show Material materials with Creep strength of 125 MPa | T851 | up to 1000 hours | ||

260 °C | 105 MPa Show Material materials with Creep strength of 105 MPa | T851 | up to 1000 hours | ||

315 °C | 41 MPa Show Material materials with Creep strength of 41 MPa | T851 | up to 1000 hours | ||

370 °C | 14 MPa Show Material materials with Creep strength of 14 MPa | T851 | up to 1000 hours | ||

Elastic modulus | 73.0 GPa Show Material materials with Elastic modulus of 73.0 GPa | T851 | AA Standards, ASTM B209, ASTM B211 | ||

73 GPa Show Material materials with Elastic modulus of 73 GPa | T851 | ||||

74.0 GPa Show Material materials with Elastic modulus of 74.0 GPa | T851 | ||||

Elongation | -195 °C | 15 % Show Material materials with Elongation of 15 % | T851 | Elongation in 50 mm | |

-80 °C | 13 % Show Material materials with Elongation of 13 % | T851 | Elongation in 50 mm | ||

3.0 % Show Material materials with Elongation of 3.0 % | T851 | AA Standards, ASTM B209, ASTM B211 | A100 | ||

4.0 % Show Material materials with Elongation of 4.0 % | T851 | AA Standards, ASTM B209 | A100 | ||

5.0 % Show Material materials with Elongation of 5.0 % | T851 | AA Standards, ASTM B209 | A100 | ||

6.0 % Show Material materials with Elongation of 6.0 % | T851 | AA Standards, ASTM B209 | A100 | ||

6.7 % Show Material materials with Elongation of 6.7 % | T851 | ||||

7.0 % Show Material materials with Elongation of 7.0 % | T851 | AA Standards, ASTM B209 | A100 | ||

8.0 % Show Material materials with Elongation of 8.0 % | T851 | AA Standards, ASTM B209 | A50 | ||

10.0 % Show Material materials with Elongation of 10.0 % | T851 | AA Standards | A50 | ||

0 °C | 12 % Show Material materials with Elongation of 12 % | T851 | Elongation in 50 mm | ||

24 °C | 12 % Show Material materials with Elongation of 12 % | T851 | Elongation in 50 mm | ||

100 °C | 15 % Show Material materials with Elongation of 15 % | T851 | Elongation in 50 mm | ||

150 °C | 17 % Show Material materials with Elongation of 17 % | T851 | Elongation in 50 mm | ||

205 °C | 20 % Show Material materials with Elongation of 20 % | T851 | Elongation in 50 mm | ||

260 °C | 21 % Show Material materials with Elongation of 21 % | T851 | Elongation in 50 mm | ||

315 °C | 55 % Show Material materials with Elongation of 55 % | T851 | Elongation in 50 mm | ||

370 °C | 75 % Show Material materials with Elongation of 75 % | T851 | Elongation in 50 mm | ||

Unlock all property charts | |||||

Fatigue strength | 103 MPa Show Material materials with Fatigue strength of 103 MPa | T851 | for 5x10⁸ cycles | ||

Plane-Strain Fracture Toughnes | 22.0 - 35.0 MPa·√m Show Material materials with Plane-Strain Fracture Toughnes of 22.0 - 35.0 MPa·√m | Typical for Wrought 2000 Series Aluminium | |||

Poisson's ratio | 0.33 [-] Show Material materials with Poisson's ratio of 0.33 [-] | Typical for Wrought 2000 Series Aluminium | |||

Shear modulus | 26.0 GPa Show Material materials with Shear modulus of 26.0 GPa | T851 | |||

Tensile strength | -195 °C | 572 MPa Show Material materials with Tensile strength of 572 MPa | T851 | up to 10000 h at temperature, at 35 MPa/min to yield strength and then at strain rate of 5%/min to fracture | |

-80 °C | 490 MPa Show Material materials with Tensile strength of 490 MPa | T851 | up to 10000 h at temperature, at 35 MPa/min to yield strength and then at strain rate of 5%/min to fracture | ||

395.0 MPa Show Material materials with Tensile strength of 395.0 MPa | T851 | AA Standards, ASTM B209, ASTM B211 | |||

400.0 MPa Show Material materials with Tensile strength of 400.0 MPa | T851 | AA Standards, ASTM B211 | |||

405.0 MPa Show Material materials with Tensile strength of 405.0 MPa | T851 | AA Standards, ASTM B209 | |||

415.0 MPa Show Material materials with Tensile strength of 415.0 MPa | T851 | AA Standards, ASTM B209 | |||

425.0 MPa Show Material materials with Tensile strength of 425.0 MPa | T851 | AA Standards, ASTM B209 | |||

455.0 MPa Show Material materials with Tensile strength of 455.0 MPa | T851 | AA Standards | |||

460.0 MPa Show Material materials with Tensile strength of 460.0 MPa | T851 | ||||

0 °C | 475 MPa Show Material materials with Tensile strength of 475 MPa | T851 | up to 10000 h at temperature, at 35 MPa/min to yield strength and then at strain rate of 5%/min to fracture | ||

24 °C | 455 MPa Show Material materials with Tensile strength of 455 MPa | T851 | |||

100 °C | 415 MPa Show Material materials with Tensile strength of 415 MPa | T851 | |||

150 °C | 338 MPa Show Material materials with Tensile strength of 338 MPa | T851 | |||

205 °C | 248 MPa Show Material materials with Tensile strength of 248 MPa | T851 | |||

260 °C | 200 MPa Show Material materials with Tensile strength of 200 MPa | T851 | |||

315 °C | 48 MPa Show Material materials with Tensile strength of 48 MPa | T851 | |||

370 °C | 30 MPa Show Material materials with Tensile strength of 30 MPa | T851 | |||

Unlock all property charts | |||||

Yield strength | -196 °C | 421 MPa Show Material materials with Yield strength of 421 MPa | T851 | up to 10000 h at temperature, at 35 MPa/min to yield strength and then at strain rate of 5%/min to fracture, RP02 | |

-80 °C | 372 MPa Show Material materials with Yield strength of 372 MPa | T851 | up to 10000 h at temperature, at 35 MPa/min to yield strength and then at strain rate of 5%/min to fracture, RP02 | ||

-28 °C | 359 MPa Show Material materials with Yield strength of 359 MPa | T851 | up to 10000 h at temperature, at 35 MPa/min to yield strength and then at strain rate of 5%/min to fracture, RP02 | ||

270.0 MPa Show Material materials with Yield strength of 270.0 MPa | T851 | AA Standards, ASTM B211 | RP02 | ||

275.0 MPa Show Material materials with Yield strength of 275.0 MPa | T851 | AA Standards, ASTM B211 | RP02 | ||

290.0 MPa Show Material materials with Yield strength of 290.0 MPa | T851 | AA Standards, ASTM B209 | RP02 | ||

295.0 MPa Show Material materials with Yield strength of 295.0 MPa | T851 | AA Standards, ASTM B209 | RP02 | ||

305.0 MPa Show Material materials with Yield strength of 305.0 MPa | T851 | AA Standards, ASTM B209 | RP02 | ||

310.0 MPa Show Material materials with Yield strength of 310.0 MPa | T851 | AA Standards, ASTM B209 | RP02 | ||

315.0 MPa Show Material materials with Yield strength of 315.0 MPa | T851 | AA Standards, ASTM B209 | RP02 | ||

340.0 MPa Show Material materials with Yield strength of 340.0 MPa | T851 | ||||

350.0 MPa Show Material materials with Yield strength of 350.0 MPa | T851 | AA Standards | RP02 | ||

24 °C | 345 MPa Show Material materials with Yield strength of 345 MPa | T851 | |||

100 °C | 324 MPa Show Material materials with Yield strength of 324 MPa | T851 | |||

149 °C | 276 MPa Show Material materials with Yield strength of 276 MPa | T851 | |||

204 °C | 200 MPa Show Material materials with Yield strength of 200 MPa | T851 | |||

260 °C | 159 MPa Show Material materials with Yield strength of 159 MPa | T851 | |||

316 °C | 41 MPa Show Material materials with Yield strength of 41 MPa | T851 | |||

371 °C | 26 MPa Show Material materials with Yield strength of 26 MPa | T851 | |||

Unlock all property charts |

Thermal

Property | Temperature | Value | Condition | Related Standards |
---|---|---|---|---|

Coefficient of thermal expansion | 2.2e-05 1/K Show Material materials with Coefficient of thermal expansion of 2.2e-05 1/K | T851 | ||

20 °C | 2.23e-05 1/K Show Material materials with Coefficient of thermal expansion of 2.23e-05 1/K | T851 | AA Standards, ASTM B209, ASTM B211 | |

100 °C | 2.23e-05 1/K Show Material materials with Coefficient of thermal expansion of 2.23e-05 1/K | T851 | AA Standards, ASTM B209, ASTM B211 | |

Unlock all property charts | ||||

Melting point | 540.0 °C Show Material materials with Melting point of 540.0 °C | T851 | ||

545.0 - 645.0 °C Show Material materials with Melting point of 545.0 - 645.0 °C | T851 | AA Standards, ASTM B209, ASTM B211 | ||

Specific heat capacity | 860.0 J/(kg·K) Show Material materials with Specific heat capacity of 860.0 J/(kg·K) | T851 | ||

Thermal conductivity | 113.0 - 172.0 W/(m·K) Show Material materials with Thermal conductivity of 113.0 - 172.0 W/(m·K) | T851 | AA Standards, ASTM B209, ASTM B211 | |

140.0 W/(m·K) Show Material materials with Thermal conductivity of 140.0 W/(m·K) | T851 |

Electrical

Property | Value | Condition | Related Standards | Comment |
---|---|---|---|---|

Electrical conductivity | 16000000.0 - 26000000.0 S/m Show Material materials with Electrical conductivity of 16000000.0 - 26000000.0 S/m | T851 | AA Standards, ASTM B209, ASTM B211 | |

17000000 S/m Show Material materials with Electrical conductivity of 17000000 S/m | T851 | Typical/derived value | ||

Electrical resistivity | 3.85e-08 - 6.25e-08 Ω·m Show Material materials with Electrical resistivity of 3.85e-08 - 6.25e-08 Ω·m | T851 | AA Standards, ASTM B209, ASTM B211 | |

5.7e-08 Ω·m Show Material materials with Electrical resistivity of 5.7e-08 Ω·m | T851 | Typical value | ||

Specific Electrical conductivity | 30.0 % IACS Show Material materials with Specific Electrical conductivity of 30.0 % IACS | T851 | Typical value |

Chemical properties

Property | Value | Condition | Related Standards |
---|---|---|---|

Aluminium | 91.5 - 93.8 % Show Material materials with Aluminium of 91.5 - 93.8 % | T851 | |

Copper | 5.8 - 6.8 % Show Material materials with Copper of 5.8 - 6.8 % | T851 | AA Standards, ASTM B209, ASTM B211 |

Iron | 0.30 % Show Material materials with Iron of 0.30 % | T851 | AA Standards, ASTM B209, ASTM B211 |

0.3 % Show Material materials with Iron of 0.3 % | T851 | ||

Magnesium | 0.02 % Show Material materials with Magnesium of 0.02 % | T851 | AA Standards, ASTM B209, ASTM B211 |

Manganese | 0.2 - 0.4 % Show Material materials with Manganese of 0.2 - 0.4 % | T851 | AA Standards, ASTM B209, ASTM B211 |

Other | 0.15 % Show Material materials with Other of 0.15 % | T851 | |

Silicon | 0.2 % Show Material materials with Silicon of 0.2 % | T851 | AA Standards, ASTM B209, ASTM B211 |

Titanium | 0.02 - 0.1 % Show Material materials with Titanium of 0.02 - 0.1 % | T851 | AA Standards, ASTM B209, ASTM B211 |

Vanadium | 0.05 - 0.15 % Show Material materials with Vanadium of 0.05 - 0.15 % | T851 | AA Standards, ASTM B209, ASTM B211 |

Zinc | 0.1 % Show Material materials with Zinc of 0.1 % | T851 | AA Standards, ASTM B209, ASTM B211 |

Zirconium | 0.1 - 0.25 % Show Material materials with Zirconium of 0.1 - 0.25 % | T851 | AA Standards, ASTM B209, ASTM B211 |

Technological properties

Property | ||
---|---|---|

Brazing | general: no brazing is known or developed | |

Corrosion properties | Stress corrosion cracking: Betriebsschäden in Gebieten mit Zugspannungen quer zur Kornstruktur, Eingeschränkte Schäden an Laborproben (T31, T351, T3510, T3511, T37), kein Schadensfall im Betrieb, eingeschränkte Schäden bei den Labortests (T81, T851, T8510, T8511), general: sufficient, in principle it should be protected | |

General machinability | General: good to acceptable | |

Workability | general (condition): poor(T31, T351, T3510, T3511), not suitable (T37, T81, T851, T8510, T8511, T87) |